From Wikipedia, the free encyclopedia - View original article
Glass fiber reinforced concrete, also known as GFRC or GRC, is a type of fiber reinforced concrete. Glass fiber concretes are mainly used in exterior building façade panels and as architectural precast concrete. Somewhat similar materials are fiber cement siding and cement boards.
Glass fiber reinforced concrete consists of high strength glass fiber embedded in a cementitious matrix. In this form, both fibers and matrix retain their physical and chemical identities, while offering a synergism: a combination of properties that can not be achieved with either of the components acting alone. In general, fibers are the principal load-carrying members, while the surrounding matrix keeps them in the desired locations and orientation, acting as a load transfer medium between the fibers and protecting them from environmental damage. In fact, the fibers provide reinforcement for the matrix and other useful functions in fiber-reinforced composite materials. Glass fibers can be incorporated into a matrix either in continuous or discontinuous (chopped) lengths.
A widely used application for fiber-reinforced concrete is structural laminate, obtained by adhering and consolidating thin layers of fibers and matrix into the desired thickness. The fiber orientation in each layer as well as the stacking sequence of various layers can be controlled to generate a wide range of physical and mechanical properties for the composite laminate. GFRC cast without steel framing is commonly used for purely decorative applications such as window trims, decorative columns, exterior friezes, or limestone-like wall panels.
|This section requires expansion. (August 2012)|
The potential for using a glass fiber reinforced concrete system was recognized by the Soviets in the 1940s.
The design of glass fiber reinforced concrete panels proceeds from a knowledge of its basic properties under tensile, compressive, bending and shear forces, coupled with estimates of behavior under secondary loading effects such as creep, thermal response and moisture movement.
There are a number differences between structural metal and fiber-reinforced composites. For example, metals in general exhibit yielding and plastic deformation, whereas most fiber-reinforced composites are elastic in their tensile stress-strain characteristics. However, the dissimilar nature of these materials provides mechanisms for high-energy absorption on a microscopic scale comparable to the yielding process. Depending on the type and severity of external loads, a composite laminate may exhibit gradual deterioration in properties but usually does not fail in a catastrophic manner. Mechanisms of damage development and growth in metal and composite structure are also quite different. Other important characteristics of many fiber-reinforced composites are their non-corroding behavior, high damping capacity and low coefficients of thermal expansion.
Glass fiber reinforced concrete architectural panels have the general appearance of pre-cast concrete panels, but differ in several significant ways. For example, the GFRC panels on the average, weigh substantially less than pre-cast concrete panels due to their reduced thickness. Their low weight decreases loads superimposed on the building’s structural components. The building frame becomes more economical.
A sandwich panel is a composite of three or more materials bonded together to form a structural panel. It takes advantage of the shear strength of a low density core material and the high compressive and tensile strengths of the GFRC facing to obtain high strength-to-weight ratios.
The theory of sandwich panels and functions of the individual components may be described by making an analogy to an I-beam. The core in a sandwich panel is comparable to the web of an I-beam, which supports the flanges and allows them to act as a unit. The web of the I-beam and the core of the sandwich panels carry the beam shear stresses. The core in a sandwich panel differs from the web of an I-beam in that it maintains a continuous support for the facings, allowing the facings to be worked up to or above their yield strength without crimping or buckling. Obviously, the bonds between the core and facings must be capable of transmitting shear loads between these two components thus making the entire structure an integral unit.
The load carrying capacity of a sandwich panel can be increased dramatically by introducing light steel framing. Light steel stud framing is similar to conventional steel stud framing for walls, except that the frame is encased in a concrete product. Here, the sides of the steel frame are covered with two or more layers of GFRC, depending on the type and magnitude of external loads. The strong and rigid GFRC provides full lateral support on both sides of the studs, preventing them from twisting and buckling laterally. The resulting panel is lightweight in comparison with traditionally reinforced concrete, yet is strong and durable and can be easily handled.